Elucidating the Mechanism of a Two-Step Spin Transition in a Nanoporous Metal-Organic Framework
Gregory J. Halder; Karena W. Chapman; Suzanne M. Neville; Boujemaa Moubaraki; Keith S. Murray; Jean-François Létard; Cameron J. Kepert; Journal of the American Chemical Society 130 (2008) 17552–17562; doi:10.1021/ja8068038

data_4108880
_publ_contact_author_address
; 
School of Chemistry
University of Sydney
NSW 2006
Australia
;
_publ_contact_author_email       c.kepert@chem.usyd.edu.au
_publ_contact_author_fax         +61-2-9351-3329
_publ_contact_author_name        'Prof. Cameron J. Kepert'
_publ_contact_author_phone       +61-2-9351-5741
_publ_section_title
;
 Elucidating the Mechanism of a Two-Step Spin Transition in a Nanoporous
 Metal-Organic Framework
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              17552
_journal_page_last               17562
_journal_paper_doi               10.1021/ja8068038
_journal_volume                  130
_journal_year                    2008
_chemical_formula_moiety         'C26 H24 Fe N6 S2, 3(C3 H6 O)'
_chemical_formula_sum            'C35 H42 Fe N6 O3 S2'
_chemical_formula_weight         714.72
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           18
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      18
_symmetry_space_group_name_Hall  'P 2 2ab'
_symmetry_space_group_name_H-M   'P 21 21 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   15.114(3)
_cell_length_b                   15.101(3)
_cell_length_c                   16.842(3)
_cell_measurement_reflns_used    6088
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      27.97
_cell_measurement_theta_min      2.419
_cell_volume                     3844.0(13)
_computing_cell_refinement       'SMART (BrukerAXS, 1997)'
_computing_data_collection       'SMART (BrukerAXS, 1997)'
_computing_data_reduction        'SAINT+ (BrukerAXS, 1997)'
_computing_molecular_graphics    'XPMA/ZORTEP, Webalb Viewer Pro 3.7'
_computing_publication_material  XCIF
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_measurement_device_type  'Bruker AXS 1000 CCD'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0280
_diffrn_reflns_av_sigmaI/netI    0.0295
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            33782
_diffrn_reflns_theta_full        28.00
_diffrn_reflns_theta_max         28.00
_diffrn_reflns_theta_min         1.21
_diffrn_standards_decay_%        0.00
_diffrn_standards_number         286
_exptl_absorpt_coefficient_mu    0.541
_exptl_absorpt_correction_T_max  0.927
_exptl_absorpt_correction_T_min  0.827
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS, Bruker 1995'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.235
_exptl_crystal_description       'rectangular rods'
_exptl_crystal_F_000             1504
_exptl_crystal_size_max          0.41
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.14
_refine_diff_density_max         0.510
_refine_diff_density_min         -0.505
_refine_diff_density_rms         0.098
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.151
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     230
_refine_ls_number_reflns         8918
_refine_ls_number_restraints     132
_refine_ls_restrained_S_all      1.175
_refine_ls_R_factor_all          0.0985
_refine_ls_R_factor_gt           0.0865
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0154P)^2^+14.4588P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1712
_refine_ls_wR_factor_ref         0.1782
_reflns_number_gt                7920
_reflns_number_total             8918
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja8068038_si_002_2.cif
_cod_data_source_block           SCOF-4(Ac)-150
_cod_original_cell_volume        3844.0(14)
_cod_database_code               4108880